SlideShare utilise les cookies pour améliorer les fonctionnalités et les performances, et également pour vous montrer des publicités pertinentes. Si vous continuez à naviguer sur ce site, vous acceptez l’utilisation de cookies. Consultez nos Conditions d’utilisation et notre Politique de confidentialité.
SlideShare utilise les cookies pour améliorer les fonctionnalités et les performances, et également pour vous montrer des publicités pertinentes. Si vous continuez à naviguer sur ce site, vous acceptez l’utilisation de cookies. Consultez notre Politique de confidentialité et nos Conditions d’utilisation pour en savoir plus.
Available online at www.sciencedirect.com Acta Materialia 59 (2011) 364–374 www.elsevier.com/locate/actamat Chemical gradients across phase boundaries between martensiteand austenite in steel studied by atom probe tomography and simulation O. Dmitrieva a, D. Ponge a, G. Inden a, J. Millan a, P. Choi a, J. Sietsma b, D. Raabe a,⇑ ´ a Max-Planck-Institut fur Eisenforschung, Max-Planck-Str. 1, 40237 Dusseldorf, Germany ¨ ¨ b Delft University of Technology, Faculty 3mE, Dept. MSE, 2628 CD Delft, The Netherlands Received 14 June 2010; received in revised form 2 September 2010; accepted 22 September 2010 Available online 18 October 2010Abstract Partitioning at phase boundaries of complex steels is important for their properties. We present atom probe tomography results acrossmartensite/austenite interfaces in a precipitation-hardened maraging-TRIP steel (12.2 Mn, 1.9 Ni, 0.6 Mo, 1.2 Ti, 0.3 Al; at.%). The sys-tem reveals compositional changes at the phase boundaries: Mn and Ni are enriched while Ti, Al, Mo and Fe are depleted. More speciﬁc,we observe up to 27 at.% Mn in a 20 nm layer at the phase boundary. This is explained by the large diﬀerence in diﬀusivity betweenmartensite and austenite. The high diﬀusivity in martensite leads to a Mn ﬂux towards the retained austenite. The low diﬀusivity inthe austenite does not allow accommodation of this ﬂux. Consequently, the austenite grows with a Mn composition given by local equi-librium. The interpretation is based on DICTRA and mixed-mode diﬀusion calculations (using a ﬁnite interface mobility).Ó 2010 Acta Materialia Inc. Published by Elsevier Ltd. All rights reserved.Keywords: Precipitation hardening; High-strength steels; TRIP; Aging; Atom probe tomography1. Introduction with the maraging (i.e. martensite aging) eﬀect [12,13]. The TRIP eﬀect exploits the deformation-stimulated transfor- Mn is among the most important alloying elements for mation of metastable retained austenite into martensitethe design of advanced high-strength steels, as it aﬀects and the resulting plasticity required to accommodatethe stabilization of the austenite, the stacking fault energy the transformation misﬁt [1–7]. The maraging eﬀect usesand the transformation kinetics [1–11]. Besides these global the hardening of the heavily strained martensite throughmechanisms which are exploited particularly in designing the formation of nanosized intermetallic precipitatessteels with transformation-induced plasticity (TRIP) and during aging heat treatment. The maraging-TRIP steelstwinning-induced plasticity (TWIP) eﬀects, Mn has very used in this work reveal the surprising property that bothlow diﬀusion rates in the austenite and a high segregation strength and total elongation increase upon aging, reachingor respectively partitioning tendency at interfaces. This an ultimate tensile strength of nearly 1.3 GPa at an elonga-context makes Mn (as well as the other elements discussed tion above 20% [12–14].in this paper) a very interesting candidate for an atomic- The studied alloy contains 12.2 at.% Mn, low carbonscale study of compositional changes across austenite/ content (0.05 at.%) and minor additions of Ni, Ti, Al andmartensite interfaces. Mo. Its microstructure after aging is characterized by the The speciﬁc material studied in this work is a precipita- presence of up to 15–20 vol.% austenite, a ﬁne martensitetion-hardened alloy that we refer to as maraging-TRIP matrix, and dispersed nanoscaled Ni–Al–Mn-enrichedsteel. It was developed by combining the TRIP mechanism zones [12–14]. Besides the increase in strength, a simulta- neous increase of ductility was found upon aging. This ⇑ Corresponding author. Tel.: +49 2116792325; fax: +49 2116792333. eﬀect is interpreted in terms of sluggish reaustenitization E-mail address: email@example.com (D. Raabe). during aging and the eﬀect of tempering of the as-quenched1359-6454/$36.00 Ó 2010 Acta Materialia Inc. Published by Elsevier Ltd. All rights reserved.doi:10.1016/j.actamat.2010.09.042
O. Dmitrieva et al. / Acta Materialia 59 (2011) 364–374 365martensite . Partial retransformation into austenite 3. Results(besides the existing retained austenite) by a reconstructivemechanism involving Mn partitioning might be responsible 3.1. Analysis of the 3-D atom probe reconstructionfor this process. In order to elucidate this transformation phenomenon, 3.1.1. Manganese distributionparticularly the role of Mn, we focus in this work on the Fig. 1a gives a microstructure overview of the maraging-analysis of nanoscale elemental diﬀusion gradients across TRIP steel after quenching and subsequent aging (48 h atabutting martensite/retained austenite phase areas. Atom 450 °C). The upper micrograph is an electron backscatterprobe tomography (APT) is a characterization technique diﬀraction (EBSD) image where the cubic martensite isthat provides three-dimensional elemental mapping with plotted green and the retained austenite red (the retainednearly atomic resolution and gives information on the austenite was already present in the as-quenched statetopology of interfaces and local chemical gradients [15– before aging [12–14]). The middle image shows a transmis-27]. We conducted APT using an advanced local electrode sion electron microscopy (TEM) micrograph with precipi-atom probe device (Imago LEAP 3000X HR). Both the tate-containing martensite and precipitate-free austenite.two phases (austenite, martensite) and the interfaces The bottom image shows an APT reproduction whichbetween them were chemically analyzed at the atomic scale. includes both martensitic and austenitic zones. Ni atomsAdditionally, statistical thermodynamic and kinetic calcu- are shown in cyan and Mn atoms in blue. The yellow iso-lations were conducted for the given initial and boundary surfaces indicate 18 at.% Mn. Note that the three imagesvalues using Thermo-Calc [28,29] in conjunction with the reveal the hierarchy of the microstructure but the individ-kinetic simulation software DICTRA [30–32] and with a ual images were not taken at precisely the positions indi-mixed-mode kinetic approach that considers ﬁnite interface cated. Fig. 1b gives a local overview of the distribution ofmobility [33,34]. the Ni and Mn atoms in the center of the APT data set pre- sented in Fig. 1a. For clarity, only a longitudinal section of2. Experimental 20 nm thickness is shown, in which only 7.8% of all detected Ni (cyan) and 1.5% of all Mn (dark blue) atoms The investigated maraging-TRIP steel with a composi- are displayed. The whole analysis volume is abouttion of 12.2 Mn, 1.9 Ni, 0.6 Mo, 1.2 Ti, 0.1 Si, 0.3 Al and 4 Â 105 nm3. Fig. 1a and b show three main zones that0.05 C (at.%) was melted and cast in a vacuum induction fur- are separated by inclined plate-like Mn accumulations.nace. Before ﬁnal age hardening, a solution treatment was Ni-rich nanoprecipitates are dispersed in the left- andperformed in Ar atmosphere at 1050 °C for 0.5 h followed right-hand areas. Besides the Ni atoms, higher amountsby water quenching. This led to a microstructure consisting of Al, Mn, and Ti were also detected in these clustersof martensite and retained austenite. Final aging was con- (Table 1). In the center part between the Mn-enrichedducted for 48 h at 450 °C. After aging the sample was plates, no precipitates appear. This observation stronglyquenched in water. Details of the alloy preparation have suggests that this zone corresponds to austenite, whereasbeen published elsewhere [12–14]. the abutting areas containing precipitates are martensitic. APT samples were prepared by electrochemical polish- Correlative TEM investigations conducted on this alloying and subsequent sharpening using a focused ion beam in the same aging state (48 h, 450 °C) support the sugges-device. Pulsed-laser APT was performed using a local elec- tion that the nanoparticles that are enriched in Ni, Altrode atom probe (LEAPe 3000X HR, Imago Scientiﬁc and Mn formed in the martensitic microstructure whileInstruments) tomograph at a specimen temperature of the retained austenite (total volume fraction about 15–2054 K. An ultrafast pulsed laser of $10 ps pulse width and vol.%) was precipitate-free [13,14] (Fig. 1a). From these532 nm wavelength was applied at a frequency of observations we conclude that the present volume probed250 kHz. The laser pulse energy was set to 0.4 nJ. The by APT contains an austenitic grain enclosed betweendetection rate (target evaporation rate) amounted to 5 two martensitic grains. Quantitative chemical analysis ofatoms per 1000 pulses. Data analysis was performed using the interfaces between austenite and martensite was per-the IVASÒ software from Imago Scientiﬁc Instruments. formed using 1-D concentration proﬁles computed overThe speciﬁc APT data set analyzed in this work contains the region of interest (transparent cylindrical units)about 70 million ions. We used an evaporation ﬁeld con- (Fig. 2a). We calculated the Mn content averaged overstant of 26 V nm–1 for the atomic reconstruction. the 0.5 nm thick cross-sections of the cylinders at a proﬁle Phase fractions and the elemental compositions in ther- step size of 0.5 nm. For both interfaces, a strong increase inmodynamic equilibrium were calculated using the software the Mn content up to 27 at.% was observed (Fig. 2b). AwayThermo-Calc . The software DICTRA [30–32] and a from the interface, the content of Mn within the austenitemixed-mode kinetic approach including ﬁnite interface amounts to about 12 at.% which is close to the averagemobility [33,34] were applied to simulate diﬀusion-con- chemical composition of the alloy. Within the bulk mar-trolled phase transformations. The simulations were per- tensite the Mn content amounts to about 10 at.%. Mnformed using the thermodynamic database TCFE6  depletion in the martensite down to 6 at.% was observedand the mobility database MOB2. close to the interface.
366 O. Dmitrieva et al. / Acta Materialia 59 (2011) 364–374 In order to exclude the contribution of the precipitates from the chemical proﬁle within the martensitic area, we separately measured the 1-D concentration proﬁles within the martensitic matrix after removing the precipitate zones from the analysis volume (described in detail below). The reason for this procedure is that the martensitic area is in itself a two-phase region consisting of martensite and pre- cipitates. Hence, we aim with this method at the separation of the martensite elemental composition and the precipitate elemental composition. These two corrected proﬁles, con- taining only the martensite composition, are included in Fig. 2b on the left-hand side in the martensitic area marked “M”. The curves are separated from the proﬁle across the interface and in the austenite (“A”). 3.1.2. Distribution of other alloying elements Fig. 3 shows the concentration proﬁles for the other alloying elements across one of the martensite/austenite phase boundary zones. The area selected is indicated by “Mn layer 2” in Fig. 2a. In addition to Mn (which is studied here in more detail owing to its relevance for high-strength steels), all other elements also reveal a strong partitioning between the two phases. While Mn is enriched by about 2.1 times within the interface boundary layer rel- ative to its average content in the alloy, Ni is accumulated 1.2 times in the same zone. All other elements are depleted in the interface zone: Ti decays by a factor of about 6.9 times relative to the average content, Al by a factor of 6.6, Mo 2.0 and Fe 1.2. Another important observation is the large chemical width of the phase boundary zone: the enrichment zone associated with the austenite/martens- ite interface extends over a length of about 20 nm normal to the boundary segment studied. 3.1.3. Chemical analysis of the nanoparticles and of the alloy matrix The nanoparticles detected in the martensite were ana- lyzed using a cluster search algorithm implemented in the 3 Fig. 1. (a) Microstructure overview of the maraging-TRIP steel after quenching and subsequent aging (48 h at 450 °C). The upper micrograph is an EBSD image where the cubic martensite is plotted green and the retained austenite red (the retained austenite was already present in the as- quenched state before aging). The middle image shows a TEM micrograph with precipitate-containing martensite and precipitate-free austenite. The bottom image shows an APT reproduction which includes both martens- itic and austenitic zones. Ni atoms are given in cyan and Mn atoms in blue. The yellow isosurfaces indicate 18 at.% Mn. Note that the three images correctly reveal the hierarchy of the microstructure but the individual images were not taken at precisely the positions indicated. (b) 20 nm thick middle layer slice through the APT reconstruction of the maraging-TRIP steel shown in (a). Ni atoms (cyan symbols) are accumulated in precipitates in the martensitic grains (left- and right-hand side). The precipitate-free austenite (right-hand center) is bordered by plate-like zones that are characterized by strong Mn enrichment (blue symbols). Red dotted lines illustrate the suggested crystallographic positions of the phase boundaries between martensite and austenite.
O. Dmitrieva et al. / Acta Materialia 59 (2011) 364–374 367 Fig. 1 (continued)Table 1(Experimental results) Elemental composition of the alloy measured globally on the as-cast sample using wet chemical analysis (total content melt) andobtained locally from the APT measurement on the specimen volume containing a martensite/austenite phase boundary of 450 °C/48 h aged steel (totalcontent APT; martensite; austenite). Enrichment factors are calculated as the relation between the elemental content within the particles to the totalcontent of element in the alloy.Chemical content, at.% Total content (melt) Total content (in APT) Martensite Austenite Total Matrix Particles Enrichment factorFe 83.71 83.21 84.38 86.82 40.32 0.48 83.53Mn 12.19 12.34 11.10 10.29 26.07 2.35 12.17Ni 1.90 2.26 2.32 0.99 25.79 11.12 2.01Ti 1.17 1.10 1.09 0.98 3.23 2.96 1.14Mo 0.58 0.60 0.60 0.62 0.27 0.45 0.60Al 0.31 0.33 0.34 0.14 4.08 12.0 0.38Si 0.10 0.16 0.15 0.14 0.24 1.6 0.16C 0.046 0.006 0.001 0.001 0 0.006Fig. 2. Quantitative chemical analysis of the interface regions between martensite and austenite (APT results). (a) Atomic map section showing both phaseboundaries. Isoconcentration surfaces for the chemical distribution of Mn atoms (blue) were plotted at 18 at.% (yellow). 1-D proﬁles along the cylindricalunits (cyan) provide chemical gradients of elements across the phase boundaries. (b) Gradients in Mn content across the phase boundaries (martensite toaustenite).IVASÒ software. For cluster identiﬁcation, the following chemical composition of the clusters is summarized inparameters as identiﬁed by the optimization procedure per- Table 1. The calculation of the enrichment factors thatformed within the cluster search algorithm were used: were determined as a relation between the content withindmax = 0.6 nm (maximal distance between the solute atoms the particles relative to the total content of the same ele-belonging to a cluster), Nmin = 50 (minimal number of sol- ments in the entire alloy reveals a strong precipitation char-ute atoms in the cluster), L = 0.57 nm (envelope distance: acter of Ni and Al atoms within the clusters. Enrichment inall non-solute ions within a distance L of solute ions are Mn and Ti was also detected in the particles. For estimat-included in the cluster), de = 0.55 nm (erosion distance: ing the chemical composition of the surrounding matrixall clustered non-solute ions within a spacing de of any (without the precipitates), the detected clusters wereion outside of its assigned cluster are removed from the removed from the overall reconstruction, and the composi-particle). The cluster search was conducted for the distribu- tion of the residual matrix volume was calculated again.tion of the Ni atoms that are enriched in the particles. The For this purpose, diﬀerent cluster search parameters were
368 O. Dmitrieva et al. / Acta Materialia 59 (2011) 364–374Fig. 3. Experimental APT results. (a) Concentration proﬁles for all elements across one of the martensite/austenite phase boundaries (see interfacereferred to as “Mn layer 2” in Fig. 2a). (b) Quantitative characterization of the enrichment or depletion of the elements within the chemical phaseboundary.Fig. 4. Compositional changes in the austenite/martensite interface region (APT results). (a) Atomic map section showing a phase boundary betweenaustenite (left) and martensite (right). Isoconcentration surfaces plotted at 18 at.% Mn (dark yellow) correspond to the highest Mn gradient and indicatesthe positions of the original and the ﬁnal phase boundaries (PB) (see text). The compositional changes at the ﬁnal PB are revealed by plottingisoconcentration surfaces for Ti (at 8 at.%), Mo (at 5 at.%), and Si (at 3 at.%). (b) Chemical composition of the Ti–Mo–Si-rich partitioning estimated fromthe APT data.used (dmax = 1.0 nm, Nmin = 50, L = 0.97 nm, de = 0.95 nm) same content and element distribution was also observedwhich allow inclusion of more material in the clusters and at the other martensite/austenite interface (not shown inensure that after exclusion of the clusters no residual material Fig. 4a). The average chemical composition within theremains. The composition of the matrix without the particles region is summarized in the table in Fig. 4b. The enrich-is presented in Table 1. ment factors reveal strong compositional increase of Ti, Mo and Si, and strong depletion of Al. The relative concen-3.1.4. Observation of compositional changes within the trations of Fe, Ti and Mo within that region are 75:17:8,martensite/austenite interface region suggesting the formation of a Laves phase, which accord- By computing the isoconcentration surfaces for all sol- ing to Thermo-Calc should be formed at a compositionute elements from the experimental data we detected of Fe 67 at.%, Ti 23 at.%, and Mo 10 at.%.changes in composition of Mo, Ti and Si in the martens-ite/austenite interface region. Fig. 4a shows isosurfaces 3.2. Thermodynamic calculationsfor Mo, Ti and Si concentrations of 5, 8 and 3 at.%, respec-tively. The position of this region overlaps with the posi- 3.2.1. Prediction of the phase equilibrium compositiontion of the isoconcentration surface plotted at 18 at.% Using Thermo-Calc, the equilibrium compositions of sta-Mn and, more speciﬁcally, corresponds to the range of ble phases at 450 °C were calculated taking into account thethe highest Mn gradient. A similar region with nearly the total nominal composition of the alloy and all possible
O. Dmitrieva et al. / Acta Materialia 59 (2011) 364–374 369Table 2Equilibrium phases at 450 °C in the investigated maraging-TRIP steel as obtained by Thermo-Calc calculations quantiﬁed in terms of molar fractions(TCFE6 database).Phase Mole fraction Fe Mn Ni Ti Mo Al Si Cbcc 0.576 95.972 3.064 0.098 0.165 0.113 0.494 0.094 –fcc 0.377 67.251 27.569 4.887 0.053 0.077 0.041 0.122 –Laves 0.046 65.911 0.763 – 22.321 11.005 – – –TiC 0.001 – – – 54.046 – – – 45.954competing phases available in the database [28,29]. The most of the nanoprecipitates were indeed associated withresults of the Gibbs energy minimization technique predicts dislocations, which supports the assumption that the pipefour phases in thermodynamic equilibrium: body-centered mechanism may strongly assist diﬀusion within the mar-cubic (bcc: ferrite/martensite), face-centered cubic (fcc: aus- tensite. In order to take into account the variation of com-tenite), TiC and a Laves phase. The calculated molar frac- position in the ferrite due to the precipitation of particles,tions for each phase and their chemical compositions are an average composition was used for the ferrite phaselisted in Table 2. It is important to point out that such calcu- (see Fig. 5b). Martensite is not included as a separate phaselation does not predict the presence of the nanosized parti- in the thermodynamic and kinetic databases as the thermo-cles due to the limited availability of thermodynamic data dynamic properties of martensite are very much the samerelated to various other possible intermetallic phases in com- as those of ferrite. Therefore, in the thermodynamic calcu-plex maraging steels. At a temperature of 450 °C, a Mn con- lations, martensite is represented as ferrite. The kinetictent of about 26.7 and 3.3 at.% is expected in the retained parameters, however, may deviate between the two phasesaustenite and in the ferrite (martensite), respectively. owing to the defect structure and distortion of the martens- ite. To date, no detailed information is available on the3.2.2. Diﬀusion simulations using DICTRA eﬀect of these conditions on possible changes in the kinetic For simulation of the kinetic behavior in the vicinity of parameters between ferrite and martensite.the martensite/austenite interface, linear cell geometry is The size of the cell is ﬁxed during the simulationappropriate . The kinetic eﬀects to be studied are con- (20 lm), whereas the interface between the two regions isﬁned to very small spatial ranges. Within this scale the mobile. The conditions at the moving interface are deter-interfaces are planar in shape and their movement is verti- mined by the local equilibrium assumption, i.e. the chemi-cal to the plane. The size of the cell was chosen as 20 lm cal potentials of all diﬀusing elements assume the same(see Fig. 5a). The cell was divided into two regions, one value in ferrite and austenite. The value of the potentialscorresponding to ferrite, the other to austenite. The space is controlled by the mass balance condition. Diﬀusion ofin each region is discretized as a linear grid. The distribu- Mn, Mo, Ni, Si and Ti atoms was considered in the calcu-tion of the grid points is chosen with a high density close lation. The simulation was performed for an aging temper-to the interface. The grid is deﬁned in terms of geometric ature 450 °C and stopped at 180,000 s (50 h).series. The compositions of ferrite and austenite were taken The composition proﬁle of Mn between ferrite and aus-according to the values determined via the APT character- tenite after an annealing time of 50 h at 450 °C is presentedization for the austenitic and martensitic matrices, respec- in Fig. 6. The interface has moved towards the ferrite side,tively. In the martensitic matrix we detected a slight Mn leaving behind an austenite layer with drastically changeddepletion down to 10.3 at.%. This can be attributed to composition. This result is in qualitative agreement withthe formation of nanoprecipitates. Within martensite, a the experimental data presented in Fig. 2b. However, thelarge number of lattice defects, particularly dislocations, width of the predicted Mn-rich interfacial layer is too smallenhance the atomic diﬀusion in this phase. Our previous and, correspondingly, the extent of the Mn depletion zoneTEM-based studies on this material [12,13] revealed that in ferrite is also relatively small. This discrepancy indicatesFig. 5. (a) Linear cell model set-up with ferrite and austenite as used in the DICTRA simulation. The spatial grid is deﬁned in terms of a geometric serieswith a high density of grid points close to the interface. (b) Composition of the austenite and ferrite phases used as input for the DICTRA simulation.
370 O. Dmitrieva et al. / Acta Materialia 59 (2011) 364–374 that the mobility of Mn in the martensitic matrix must be higher than it is in ferrite. Therefore, the simulations were repeated with increased mobilities of the elements in the ferrite. The results of the simulations with a factor 12 and 45, respectively, for the enhanced mobilities in mar- tensite are shown in Fig. 7. The result in Fig. 7b (45 times enhanced Mn mobility in martensite) is in excellent agree- ment with the experimental results in Fig. 2b. This applies for the depletion proﬁle of Mn in the martensite and also for the Mn-enriched interface zone. In view of this good agreement, the proﬁles of the other elements should also be analyzed. Fig. 8a shows the com- position proﬁles of some of the elements for a mobility fac- tor of 45. Fig. 8b presents the predicted enrichment or depletion of the other elements, respectively, in the same way as for the experimental results. The partitioning ten-Fig. 6. DICTRA calculation of the Mn distribution at the martensite/austenite phase boundary. Martensite is thermodynamically and kineti- dencies of the elements are the same as observed in thecally treated as ferrite. The calculation was done for 450 °C (aging experiment (compare Figs. 3a and b and 8a and b). Thetemperature). The result is shown for the 180,000 s time step (50 h). predicted enrichment of Mn and Ni and the depletion of Mo within the interfacial austenite layer are in good quan- titative agreement with the experiments. For Ti and Si, the decrease is less pronounced in the simulation than in the experiment. We estimated the mean diﬀusion paths of Mn atoms in both phases using the diﬀusion coeﬃcients obtained for 450 °C using DICTRA (Mob2 database). The diﬀusion con- stant of Mn atoms in a bcc iron matrix (ferrite) was Dbcc = 1.75 Â 10À22 m2 s–1 and in the fcc iron matrix Dfcc = 5.86 Â 10À24 m2 s–1. The mean diﬀusion path k of Mn atoms for an aging time of t = 48 h was calculated using the volume diﬀusion equation for cubic metals: k = (6tD)½. The mean diﬀusion path of Mn atoms in the bcc lattice was about 13 nm and in the fcc lattice only about 2.5 nm. Thus, the diﬀusion length of Mn in bcc is signiﬁcantly larger than in the fcc lattice. When correcting the mobility of the atoms by a factor of 45, as explained above, the diﬀusion constant in ferrite (which can be then treated as martensite) is 7.56 Â 10À21 m2 s–1. For this case, the mean diﬀusion path of Mn in bcc increases from 13 to about 90 nm. 4. Discussion 4.1. Phase boundary motion with inﬁnite interface mobility in the DICTRA approach The global equilibrium calculated with Thermo-Calc (see Table 2) predicts a high amount of Mn in the retained austenite (27.6 at.%) and a low value (3 at.%) in ferrite. Hence, during aging a redistribution of Mn is expected. However, the global equilibrium only indicates the long term trends. The actual situation at the phase boundary is controlled by a local equilibrium. It is not possible to visualize graphically equilibria in multicomponent systems. Therefore, the following discus-Fig. 7. DICTRA calculation of the Mn distribution at the martensite/austenite interface. Martensite is thermodynamically and kinetically sion will be done considering only three components: Fe,treated as ferrite, but the mobility of the elements is increased by a factor Mn and Ni. Fig. 9 shows the ternary phase diagram atof 12 (a) and 45 (b), respectively. 450 °C. The initial compositions of martensite (ﬁlled
O. Dmitrieva et al. / Acta Materialia 59 (2011) 364–374 371Fig. 8. Results of DICTRA calculations. (a) Composition proﬁles of all elements included in the DICTRA simulation. (b) Quantitative characterization ofthe calculated proﬁles. (c) Element contents at the new interface between martensite and austenite at 450 °C for the given global composition. than in the matrix. The range of possible local equilibrium tie-lines is thus conﬁned to those originating from Ni con- centrations in martensite below the value in the a-matrix, a=c i.e. xNi < xa . This composition range is marked in Fig. 9 Ni by a bold phase boundary. The operating local equilibrium tie-line is deﬁned by the ﬂuxes of Ni and Mn. The interface displacement caused by these ﬂuxes must be the same for every diﬀusing element. The resulting operating local tie- line is indicated in Fig. 9, showing the diﬀerence to that of global equilibrium. Due to the low diﬀusivity in austenite, the ﬂuxes lead to an interface displacement towards martensite. The layer of increased Mn is the result of the partitioning imposed by the local equilibrium tie-line during the formation of aus- tenite. Epitaxial formation of this aging-induced austenite at the phase boundary of the existing austenite is likely. The overall agreement between experiment and simula- tion is very good. There is a slight diﬀerence in the Mn composition at the martensite boundary though. The experiments yield a value of about 5–6 at.% Mn, whileFig. 9. Isothermal section of the Fe–Mn–Ni ternary system. The starting the simulation gives a value of 3 at.%. There are two pos-composition of austenite (ﬁlled circle) and martensite (ﬁlled square) are sibilities to explain this diﬀerence. (i) It could be an eﬀect ofindicated. The global equilibrium tie-line is shown as a broken line. The the resolution of the experiment. The transition from thebold part of the ferrite phase boundary indicates the range of possiblelocal equilibrium tie-lines. low concentration at the martensite boundary to the very high concentration at the austenite interface occurs shar- ply. It is, therefore, plausible that close to this abrupt tran-square) and austenite (ﬁlled circle) are within the two-phase sition the Mn signal is slightly contaminated by theregion a + c. The global equilibrium tie-line is shown by a elevated Mn concentration, leading to a slightly increaseddotted line. The slope of the tie-lines indicates that at the composition close to the boundary. (ii) It could be due toaustenite phase boundary the level of both Mn and Ni the ﬁnite mobility of the interface. The local equilibriummust be higher than in the matrix. Conversely, the level approach implies that the interface can move freely. Aof Mn and Ni at the martensite boundary must be lower ﬁnite mobility of the interface (see details in the next
372 O. Dmitrieva et al. / Acta Materialia 59 (2011) 364–374 velocity, can be simulated for binary Fe–Mn on the basis of two assumptions . The ﬁrst one is that the driving force is proportional to the deviation from equilibrium: DG ¼ vðxac Þ À xa Mn Mn ð2Þ where the indices ac denote the equilibrium concentration in the a-phase (martensite) in equilibrium with c (austen- ite), and xa is the Mn concentration in martensite at the Mn interface. In the case of partitioning Mn, the proportional- ity factor v is negative. The second assumption is that the diﬀusion in the parent martensitic a-phase leads to a con- centration proﬁle that can be described by an exponential function: z xMn ¼ x0 þ ðxa À x0 Þ exp À Mn ð3Þ z0 Fig. 10. Velocity of the interface a/c as a function of time. with the spatial coordinate z = 0 at the interface. The width parameter z0 follows from the values of M and D and thesection) leads to a slower interface velocity than that given equilibrium and overall (x0) concentrations . Diﬀusionby the local equilibrium. Consequently, the boundary con- of Mn in the austenite is so slow that it can be neglected.dition has to be adapted such that the mass balance is in The experimental proﬁle in Fig. 2b shows a Mn concen-accordance with the velocity. This eﬀect, however, should tration in the a-phase at the interface of 5–6 at.%, which isbecome more relevant at rather high interface velocities. slightly larger than the equilibrium value of 3.3 at.%. ThisIn the present case of low temperature the interface velocity would imply a deviation from local equilibrium. Using theis small (see Fig. 10). This velocity range is more than six value of the interface mobility M as an adaptable parame-orders of magnitude smaller than usual velocities occurring ter and the same enhanced Mn diﬀusivity (factor 45) asduring the transition between austenite and ferrite at tem- used in the DICTRA simulations above, the Mn proﬁleperatures of about 700 °C or higher. We anticipate, there- in the martensitic phase can be adequately reproducedfore, that the ﬁnite interface mobility eﬀect might play a (Fig. 11). The ﬁnal proﬁle (t = 180,000 s) is given, but alsosecond-order role in the current case as discussed in more an intermediate stage, after 28,000 s. It is revealed that thedetail in the next section. deviation from equilibrium is larger in the earlier stages of the transformation. The calculations were conducted for a4.2. Phase boundary motion with ﬁnite interface mobility in value of v = –12.8 kJ mol–1, determined with Thermo-the mixed-mode approach Calc, and a mobility of M = 2 Â 10–21 m4 J–1 s–1 at T = 450 °C. The simulated results reveal an excellent The simulation of a partitioning phase transformationwith DICTRA as outlined above is based on the assump-tion that Mn diﬀusion is controlling the transformationkinetics. In a more generalized mixed-mode approach[33,34] the motion of the interface during the transforma-tion is deﬁned by its velocity, v, given by:v ¼ MDG ð1Þwhere DG is the free-energy diﬀerence between the phases,acting as the driving force for transformation, and M is theinterface mobility. In the purely diﬀusion-controlled trans-formation, such as discussed above, M is assumed to beinﬁnite, which means that the interface instantaneously re-acts to any deviation of the local concentration from equi-librium, thus restoring the local equilibrium. If M is ﬁnite,however, a certain balance is established between diﬀusion(in the case of Mn in a increasing the interface concentra-tion, which increases the driving force) and interface mo- Fig. 11. Results of the mixed-mode predictions of the Mn proﬁle across the austenite/martensite interfaces. In contrast to the DICTRA simula-tion (decreasing the Mn concentration at the interface, tion, here the interface mobility is taken into account . The mixed-which decreases the driving force). For given values of M mode simulation results for two aging times (red points: 28,000 s; yellowand the diﬀusivity D, the resulting value of the interface points: 180,000 s) are plotted together with the experimental data (red andconcentration, and thus of the driving force and the black lines, see Fig. 2b).
O. Dmitrieva et al. / Acta Materialia 59 (2011) 364–374 373agreement with the experiments (Fig. 11). The mobility The partitioning at the martensite/austenite interfacevalue, however, is distinctly smaller than the mobility data leads to the formation and growth of a new austenite layerfor the standard c ? a transformation around T = 800 °C, on the existing retained austenite with drastically changedwhen extrapolating with the commonly used activation composition compared to the bulk. It is to be expected thatenergy for the mobility of 140 kJ mol–1. such a layer will have an eﬀect on the mechanical properties. The mixed-mode approach uses the interface mobility as In the present case, this layer is likely to be one of the micro-an adaptable parameter. This approach is particularly use- structural changes during aging that might be responsibleful in cases where the transition is not fully controlled by for the unexpected increase in ductility after the annealingdiﬀusion. In such cases the local chemical equilibrium con- treatment . The other contribution for increasing thedition cannot be fulﬁlled. Instead, a diﬀerence in chemical ductility stems from the tempering of the martensitic matrixpotentials exists at the interface which provides the Gibbs during annealing and was reported elsewhere .energy required for the motion of the interface. If the inter- By using the advanced APT technique we gained deepface mobility is known and does act as a limiting kinetic insights into the chemical nature and dynamics of the mar-factor, it may play an essential role in the formation of tensite/austenite phase boundary during aging. The theory-the overall microstructure and hence should be included assisted 3-D chemical analysis at the nanoscale providesin the corresponding predictions. signiﬁcant enhancement of our understanding of partition- ing aﬀects and their relationship to phase transformation4.3. Comparison and conclusions from the two simulation kinetics in multiphase steels.methods Appendix A. Supplementary material The Mn distributions predicted by the calculationsrevealed diﬀusion of Mn from the ferritic phase towards Supplementary data associated with this article can bethe austenitic matrix and the accumulation of Mn at the found, in the online version, at doi:10.1016/j.actamat.2010.interface between these two regions. The composition pro- 09.042.ﬁles obtained experimentally agree with the simulations pro-vided that the mobilities of all alloying elements inmartensite are increased compared to ferrite (by a factor Referencesof 45, Fig. 7b). This applies to both types of simulation  Patel JR, Cohen M. Acta Metall 1953;1:531.approaches, i.e. DICTRA [30–32] and mixed-mode [33,34].  Bhadeshia HKDH, Edmonds DV. Metall Trans 1979;10A:895.Such an enhanced diﬀusion in martensite can be attributed  Takahashi M, Bhadeshia HKDH. Mater Trans JIM 1991;32:689.to a high defect concentration (e.g. misﬁt dislocations  Jacques PJ, Girault E, Catlin T, Geerlofs N, Kop T, van der Zwaag S,introduced through the transformation) in martensite. Pipe et al. Mater Sci Eng 1999;A273–275:475.diﬀusion might therefore be one reason for this enhanced  De Meyer M, Vanderschueren D, De Cooman BC. ISIJ Int 1999;39:813.diﬀusion [12–14].  Traint S, Pichler A, Hauzenberger K, Stiaszny P, Werner E. Steel Res So far it is not clear whether the higher mobility is valid Int 2002;73:259.for martensite in general or if this holds only in the neigh-  Zaeﬀerer S, Ohlert J, Bleck W. Acta Mater 2004;52:2765.borhood of the phase boundary which may act as a source  Brux U, Frommeyer G, Grassel O, Meyer LW, Weise A. Steel Res ¨ ¨of vacancies and provides high local dislocation densities in 2002;73:294.  Tomota Y, Strum M, Morris JW. Metall Mater Trans 1986;17A:537.its vicinity . More experimental information is needed  Song R, Ponge D, Raabe D, Kaspar R. Acta Mater 2004;53:845.to elucidate this point.  Song R, Ponge D, Raabe D. Acta Mater 2005;53:4881.  Raabe D, Ponge D, Dmitrieva O, Sander B. Scripta Mater5. Conclusions 2009;60:1141.  Raabe D, Ponge D, Dmitrieva O, Sander B. Adv Eng Mater 2009;11(7):547. We studied compositional variation phenomena on  ´ Ponge D, Millan J, Dmitrieva O, Sander B, Kostka A, Raabe D. In:martensite/austenite interfaces in a maraging-TRIP steel. Proc 2nd int symp steel sci (ISSS 2009). Kyoto: The Iron and SteelWe placed particular attention on the partitioning of Mn Institute of Japan; 2009. p. 121.at these interfaces using 3-D atom probe analysis in con-  Cerezo A, Godfrey TJ, Smith GDW. Rev Sci Instrum 1988;59:862.junction with Thermo-Calc, DICTRA and mixed-mode  Blavette D, Deconihout B, Bostel A, Sarrau JM, Bouet M, Menand A. Rev Sci Instrum 1993;64:2911.simulations (where the latter also includes the heterophase  Miller MK, Cerezo A, Hetherington MG, Smith GDW. Atom probeinterface mobility). The local boundary condition at the ﬁeld ion microscopy. Oxford: Oxford University Press; 1996.interface leads to the diﬀusion of Mn in martensite  Thuvander M, Miller MK, Stiller K. Mater Sci Eng A 1999;270:38.towards austenite. The chemical gradients of Mn predicted  Miller MK. Atom probe tomography analysis at the atomicby DICTRA at the phase boundary revealed a good quan- scale. New York: Kluwer Academic/Plenum; 2000.  Kelly TF, Miller MK. Rev Sci Instrum 2007;78:031101.titative correlation to the experimental ﬁndings. The diﬀu-  Seidman D. Annu Rev Mater Sci 2007;37:127.sion behavior of other alloying elements such as Ni, Ti  Miller MK, Forbes RG. Mater Charact 2009;60:461.and Mo could also be reproduced in the dynamic  Marquis EA, Miller MK, Blavette D, Ringer SP, Sudbrack CK,simulation. Smith GDW. MRS Bull 2009;34:725.
374 O. Dmitrieva et al. / Acta Materialia 59 (2011) 364–374 Pereloma EV, Stohr RA, Miller MK, Ringer SP. Metall Mater Trans  Thermodynamic database TCFE6 – TCS Steels/Fe-Alloys Database, 2009;40A:3069. Version 6.2, Thermo-Calc Software, www.thermocalc.com. Sauvage X, Lefebvre W, Genevois C, Ohsaki S, Hono K. Scripta ˚  Borgenstam A, Engstrom A, Hoglund L, Agren J. J Phase Equilib ¨ ¨ Mater 2009;60:1056. 2000;21:269. Al-Kassab T, Wollenberger H, Schmitz G, Kirchheim R. Tomogra- ˚  Crusius S, Inden G, Knoop U, Hoglund L, Agren J. Z Metallk ¨ phy by atom probe. In: Ruhle M, Ernst F, editors. High resolution ¨ 1992;83:673. imaging and spectroscopy of materials. Springer series in materials  Franke P, Inden G. Z Metallk 1997;88:917. science, vol. 50. Berlin: Springer-Verlag; 2000.  Bos C, Sietsma J. Scripta Mater 2007;57:1085. Choi P, da Silva M, Klement U, Al-Kassab T, Kirchheim R. Acta  Sietsma J, van der Zwaag S. Acta Mater 2004;52:4143. Mater 2005;53:4473.  Calcagnotto M, Ponge D, Raabe D. Mater Sci Eng A 2010;527:2738. Thermo-Calc Users’ Guide, Version R. Stockholm: Thermo-Calc ´  Ponge D, Millan J, Dmitrieva O, Sander B, Kostka A, Raabe D. Proc Software AB and Foundation of Computational Thermodynamics; 2nd int symp on steel science (ISSS 2009). Kyoto: The Iron and Steel 1995–2006. Institute of Japan; 2009. p. 121.